DESIGN OF LAMINATES FOR INPLANE LOADING


 Morris Clark
 1 years ago
 Views:
Transcription
1 DESIGN OF LAMINATES FOR INPLANOADING G. VERCHERY ISMANS 44 avenue F.A. Bartholdi, Le Mans, France SUMMARY This work relates to the design of laminated structures primarily loaded in membrane, such as pressure vessels. It derives complete formulas, i.e. valid for any loading and any laminate, and without any approximation. Using the so called material ratio and the loading ratio, the design criterion takes a very simple form, equating the two ratios. Keywords: design, laminate, netting theory, polar description of anisotropy, anisotropy. INTRODUCTION Structures primarily loaded in membrane, such as cylindrical pressure vessels, must certainly been considered as the simplest case for design. However even for such cases, the tools available to the designer are on one side the netting theory (NT), which provides explicit design factors but is known to be approximate, and on the other side the classical laminated plate theory (CLPT), which is a precise analysis method, but so requires an iterative process to contribute to a design. As the CLPT in its usual form involves huge algebraic manipulations, it is not possible to derive explicit formulas even for simple cases such as pressurized tubes and only numerical computations can be done. These numerical applications of the CLPT are of course very easy to do and show discrepancy between this CLPT and the netting theory but might not reveal the significant factors for the design. Surprisingly, no work seems to have faced this question of significant parameters until 2002 when Evans and Gibson [1] gave a clear insight into the problem. In order to reveal the factors involved, they succeeded in developing explicit formulas based on the CLPT and compared them to the netting analysis for balanced angleply laminated tubes with hooptoaxialstress ratio of 2:1. They have shown that part of the netting theory can be retained (the principal strains of the plies should be equal), while other parts need to be corrected and they gave a correction formula for the optimal ply angle. Although they had to do lots of tedious algebraic manipulations (Evans [2]), their formulas do not solve exactly the CLPT equations, due to the cumbersome algebra involved in the theory, so their results for the correction in the angle still retain a difference with full calculation. In the numerical examples they published, this correction is shown to be small, however its small value is not guaranteed for other cases and the challenge for an exact CLPT solution remains. To summarize, the limitations of the paper of Evans and Gibson are the following: i) they limited to angleply laminates, ii) they limited to a 2:1 ratio for the principal stresses, iii) their formulas are approximate.
2 METHODOLOGY AND HYPOTHESES For many years, the author has developed the socalled polar method for twodimensional continuum mechanics, using as variables the polar parameters, which are complex linear combinations of the Cartesian components of the stress, strain, stiffness, compliance or other tensors. Among other features, it provides an efficient description of plane anisotropy. So it is useful for twodimensional anisotropic systems such as composite materials. Specially, using these parameters, the CLPT receives an equivalent but simpler form, which makes possible many explicit algebraic developments otherwise intractable. From this, many applications can be derived for analysis and also for design of composites (see for instance [3]). This method was used in the present research, with the aim to improve the results of Evans and Gibson, and suppress their drawbacks. In this part of the paper, we will first describe the loading, geometric and material hypotheses of the study, present some important points of the polar method, then introduce two ratios which are relevant for the present research. In the next part, rules of design will be given, and the design criterion will be derived from them. Structural hypotheses We limit to the simplest conditions for the structure to be designed. Material and geometric hypotheses: the structure is or behaves like a laminated plate. with zero coupling stiffnesses and orthotropic membrane stiffnesses. We will specially consider laminates made of identical plies. Loading hypotheses: the structure is loaded in membrane, with uniform membrane forces N ij. The principal loads are N 1 and N 2, and we limit to the cases with N 1 > N 2 > 0. These hypotheses are those of the netting theory, and notably apply to pressure vessels. Extensions can be made but are not presented here as they make more intricate the discussion, which might conceal the principles of the method, that we want to emphasize. Basics of the polar method Complete equations can be found in [3]. A simpler form is sufficient in the present study. They are presented here in the case of orthotropy and in the principal axes of stress, strain or stiffness: for the stresses or membrane forces, they are obtained from the principal values with major principal axis along direction 1 as: 2 T N 1 N 2 2 R N 1 N 2 and similarly for the strains: 2 t r 1 2
3 for membrane stiffnesses with major principal axis in direction 1, they are: 8 T 0 A A A 1212 A A A 1122 A R 0 A A A 1212 A A 1111 A 2222 Similar formulas hold for ply stiffnesses and for compliances. Loading ratio A loading ratio is defined from the principal membrane forces N 1 > N 2 > 0 as: R T N 1 N 2. N 1 N 2 This quantity will prove to be more relevant to structural design than the more usual ratio N 1/ N 2 (which is the hooptoaxialstress ratio for tubes studied by Evans and Gibson). With the assumed values for the principal loads N k, this material ratio is positive and less than 1. It equals 1/3 in the classical case of cylindrical pressure vessel with hooptoaxialstress ratio equal to 2. Material ratio for the laminate With A ijkl being the inplane stiffnesses, the (inplane) orthotropy axes of the laminate are (1, 2) with the first axis along the direction of the major stiffness: A 1111 > A A material ratio is then defined from two of the polar parameters, as: A 1111 A 2222 A A 1122 A It should be noted that this material ratio does not involve the shear stiffness A Material ratio for a ply A material ratio for any ply is defined similarly from the stiffnesses Q ijkl in the material orthotropy axes (L, T) of the ply : Q LLLL Q TTTT Q LLLL 2Q LLTT Q TTTT This ratio can also be expressed with the compliances S ijkl in the same material orthotropy axes (L, T) or the engineering constants, longitudinal and transverse Young's moduli and, and principal (major) Poisson's ratio ν LT : Q LLLL Q TTTT Q LLLL 2Q LLTT Q TTTT S TTTT S LLLL S LLLL 2 S LLTT S TTTT E 2 LT Notice that this material ratio does not involve the shear property in the orthotropy axes.
4 OVERALL DESIGN PROCESS Design process is split in two steps: first at the laminate level, an overall material satisfying the loading conditions is built, and second, a convenient stacking giving the required overall properties is searched for. Both steps involve the ratios introduced above. Overall design rules We use as overall design criterion the following empirical rules, closely related to the guidelines of the netting analysis: i) select an orthotropic laminate with the major principal axis of stiffness aligned with the major principal axis of the loads, ii) select the material so that the strain is isotropic. Design based on these rules will be consequently called orthotropic isostrain design. Comments of the overall design rules These two rules are neither arbitrary nor obvious. Notice that they do not refer to a definite objective, and are not derived theoretically but are empirical, and so have to be assessed from their consequences. However some rationale is of course behind them. Starting with the meaning of the first rule, it is certainly common sense to retain orthotropic materials with axes aligned with the directions of principal stresses: as the stresses (being a second order tensor) have two orthogonal directions of symmetry, so should have the overall stiffnesses, i.e. the material should be orthotropic (for inplane stiffness properties). Further, the first rule requires that the major orthotropy axis should be along the highest stress and the minor along the lowest stress (remember that the major stiffness is not always along the major stiffness axis, as it may be offaxis, however the stiffness along the major orthotropy axis is always highest than that along the minor orthotropy axis). This point may appear questionable when comparing to the principles of the netting theory, which aims to optimize the structural strength (and in fact cannot meet exactly its assumptions and its aim), while the present formulation appears to rest on elastic behaviour rather to strength behaviour: it is a fact that for an arbitrary orthotropic material, strength and stiffness may differ in orientation and variation. Results for laminates will justify afterwards this rule together with the second rule. As a consequence of the first rule, the strains have the same principal axes than the stresses and stiffnesses, but the major strain may be along any of the principal axes. The second rule settles this point as its meaning is the following: the material should be strained at the same level in any of the principal axes, and consequently in any direction. This second rule is specially relevant for laminates made of identical plies. According to the CLPT, while the state of strain (for membrane loading) is the same through the thickness in the structure axes, it generally varies from ply to ply in the local axes (principal axes of the plies), and so the state of stress in each ply depends on the ply
5 orientation (whatever the axes considered). Only in the case of an isotropic state of strain, the strains are the same in every ply whatever the axes, and consequently the states of stress are the same in the local axes of all the plies: then, every ply is in the same state of strain and stress and so contributes equally to the structural behaviour, which is certainly a good design (and probably an optimal design). Formula of the overall design criterion Translating the design rules in equations is quite simple using the polar parameters. For an orthotropic material loaded in its symmetry axes, the stressstrain relationship, expressed in these symmetry axes with polar parameters, writes: T 4 t 4 r R 4 t 2 T 0 R 0 r Then we have to state that the overall strain is isotropic, that is: r 0 Eliminating t, this gives the design criterion, which expresses simply as the equality of the load and material ratios defined above: R T. The reader can check that this can be derived using the Cartesian components in the orthotropy axes, at the cost of more algebra. STACKING DESIGN PROCESS The previous step of design has defined an overall condition for the material: it must be orthotropic for inplane stiffness, with a fixed value of its material ratio. The next step will be to find stacking sequences meeting these requirements. As an orthotropic laminate possesses 4 independent inplane stiffness parameters, while the material ratio involves only 2 of these parameters, it can be guessed that there might be several solutions. In the following, we examine the common (and simplest) case when the laminate is made of identical plies. Polar method applied to CLPT For laminates made of identical plies, the CLPT equations receive a very simple form with the polar parameters (see [3]). We limit here to the orthotropic case useful for the present research. In this case the 4 polar inplane stiffness parameters have very simple expressions as functions of the polar parameters of the ply. Specially: T t 1 t R 1 cos 2 N k k 1 N
6 where t is the laminate thickness, N is the number of layers and θ k the orientation of the k layer. Consequently, the material ratio of the laminate is equal to the material ratio for the plies /, multiplied by a weighting factor: 1 N N cos2 k k1 It should be noticed that the weighting factor is always less than one. Stacking design equation Substituting in the last equation the value of the loading ratio gives the design equation: R T 1 T N cos 2 1 N k k 1 This equation involves three quantities, the loading ratio of the structure, the material ratio of the ply, and the weighting factor of the stacking sequence. Comments of the stacking design equation The conditions of applicability of our design process appear from this stacking design equation. As the weighting factor is less than 1, solutions can be expected only when: the loading factor should be less than the ply material factor and be at most equal, in which case the only possible solution is a unidirectional material. It can be shown from stability consideration that the material ratio of any material is also less than 1. Table 1 shows typical values for usual unidirectional composites. Table1 : Typical values of the ply material ratio / and polar stiffness parameters for unidirectional reinforcement (T 0,, R 0, in GPa). Material (V f 60%) / T 0 R 0 Eglass /epoxyde HTcarbon /epoxyde HMcarbon /epoxyde The material ratio has two effects. First, when it increases, the range of possible loading is increased too. As said above, the loading ratio range extends to the value of the material ratio, but the effect appears even larger when considering the ratio of the
7 principal stresses instead of the loading ratio. For instance, changing from glass/epoxy plies to HM carbon/epoxy plies increases the material ratio by 40%, and so is the loading ratio range, while the range for the principal stresses ratio is increased by 140%, from 3.8 up to 9. It also can be shown that when the material ratio increases, the formulas get closer to the netting analysis results, and when it goes up to 1, all the formulas reduce to the netting analysis. Using micromechanics formulas of prediction of elastic properties of UD shows that the material ratio is closely dependent on the reinforcementtomatrixstiffness ratio (such as E f /E m ): when this ratio increases, so does the material ratio / of a unidirectionally reinforced ply, up to the limiting case of a very soft matrix (for instance, rubber reinforced with steel fibres), with the ratio going up to 1. Plies reinforced with balanced fabrics have a zero material ratio and cannot be used in our design method. Plies reinforced with unbalanced fabrics have generally a low material ratio, limiting the range of loading they can efficiently carry. When the conditions of applicability are met, several solutions generally exist. The weighting factor should receive a fixed value equal to the loading ratio divided by the ply material ratio, and as it includes an unspecified number N of parameters θ k, an infinite number of solutions exist theoretically. Practical conditions on the number N and the angles values reduce the effective solutions. APPLICATION EXAMPLES To go further, the practical field of design parameters must be specified. Angleply and crossply laminates are of interest. Design of cylindrical pressure vessel is also of major importance for its practical applications as well as for comparison purpose with the netting theory and the Evans and Gibson results. Design with angleply laminates Angleply laminates with layers at ±β (or filament winding in these same directions) are defined by a unique parameter and the design equation writes: cos 2 R T This equation can be solved in seconds with a pocket calculator, to give the optimal angle in agreement with the CLPT. The influence of the significant factors can be check easily. The design angle ±β 0 of the netting theory is given by the limit case when the material ratio equals 1: cos 2 0 R T
8 It appears that cos 2 cos 2 0 so the exact angle is closer to the major stress direction than predicted by the netting theory. A quantitative comparison between these angle values can be obtained by Taylor expansion up to the second order in the quantity (  )/. It gives: 1 1 T /R T 0 1 T /R or using the principal Young's moduli and Poisson's ratio: 1 0 T /R LT 1 1 T / R third order 1 LT third order Design with crossply laminates Crossply laminates are also defined by only one parameter 0 < q < 1, the percentage q of layers at 0, with 1q layers at 90. The design equation writes: 2 q 1 R T So the percentage of plies at 0 should be higher than that indicated by the netting theory, which is such as 2 q 0 1 R /T. Design of cylindrical pressure vessel For cylindrical pressure vessels, N 1 2 N 2, so T 3R. These values in the formulas derived above for angleply laminates define the exact value of the helical angles at which such cylindrical pressure vessels must be wound, angles which are closer to the hoop direction than predicted by the netting theory. The approximate formula derived by Evans and Gibson writes: LT while the present analysis gives: LT LT third order The main difference comes from the term instead of , which appears in the denominator of the Evans and Gibson formula. It explain about 90% of the difference they observed with the numerical results they computed from the CLPT. With the second order terms (in the parentheses) of the present analysis, the CLPT values are recovered exactly.
9 CONCLUSION Within the conditions of applicability of the present approach, all the limitations of the analysis of Evans and Gibson are relieved and explicit design formulas for any state of stress and stacking sequence can be derived. A further step in this research will be to study the stability of solutions obtained. References 1. J T Evans and A G Gibson, 2002, Composite angle ply laminates and netting analysis, Proc. R. Soc. Lond., Vol A 458, pp J T Evans, 2007, private communication ( dated July 6 th, 2007). 3. G Verchery, 1999, Designing with anisotropy, keynote lecture, Twelfth International Conference on Composite Materials (ICCM12), 59 July, Paris.
Composite angle ply laminates and netting analysis
10.1098/rspa.2002.1066 FirstCite epublishing Composite angle ply laminates and netting analysis By J. T. Evans and A. G. Gibson School of Mechanical and Systems Engineering, University of Newcastle upon
More informationTHE NETTING ANALYSIS AS A LIMIT CASE OF THE LAMINATED STRUCTURE THEORY
THE NETTING ANALYSIS AS A LIMIT CASE OF THE LAMINATED STRUCTURE THEORY G. Verchery Pluralis, SaintÉtienne, France Georges.Verchery@m4x.org Keywords: netting analysis, classical laminated plate theory,
More informationModule6: Laminated CompositesII. Learning Unit1: M6.1. M 6.1 Structural Mechanics of Laminates
Module6: Laminated CompositesII Learning Unit1: M6.1 M 6.1 Structural Mechanics of Laminates Classical Lamination Theory: Laminate Stiffness Matrix To this point in the development of classical lamination
More informationLAMINATION THEORY FOR THE STRENGTH OF FIBER COMPOSITE MATERIALS
XXII. LAMINATION THEORY FOR THE STRENGTH OF FIBER COMPOSITE MATERIALS Introduction The lamination theory for the elastic stiffness of fiber composite materials is the backbone of the entire field, it holds
More informationComposite Structures. Indian Institute of Technology Kanpur
Mechanics of Laminated Composite Structures Nachiketa Tiwari Indian Institute of Technology Kanpur Lecture 23 Analysis of an Orthotropic Ply Lecture Overview Introduction Engineering constants for an 2
More informationQUESTION BANK Composite Materials
QUESTION BANK Composite Materials 1. Define composite material. 2. What is the need for composite material? 3. Mention important characterits of composite material 4. Give examples for fiber material 5.
More informationDESIGN OF COMPOSITE LAMINATED STRUCTURES BY POLAR METHOD AND TOPOLOGY OPTIMISATION
DESIGN OF COMPOSIE LAMINAED SUCUES BY POLA MEOD AND OPOLOGY OPIMISAION A. Jibawy,,3, C. Julien,,3, B. Desmorat,,4, (*), A. Vincenti UPMC Univ Paris 6, UM 79, Institut Jean Le ond d Alembert B.P. 6 4, place
More informationModule III  Macromechanics of Lamina. Lecture 23. MacroMechanics of Lamina
Module III  Macromechanics of Lamina Lecture 23 MacroMechanics of Lamina For better understanding of the macromechanics of lamina, the knowledge of the material properties in essential. Therefore, the
More informationConstitutive Equations
Constitutive quations David Roylance Department of Materials Science and ngineering Massachusetts Institute of Technology Cambridge, MA 0239 October 4, 2000 Introduction The modules on kinematics (Module
More information3D and Planar Constitutive Relations
3D and Planar Constitutive Relations A School on Mechanics of Fibre Reinforced Polymer Composites Knowledge Incubation for TEQIP Indian Institute of Technology Kanpur PM Mohite Department of Aerospace
More informationHygrothermal stresses in laminates
Hygrothermal stresses in laminates Changing environment conditions (temperature and moisture) have an important effect on the properties which are matrix dominated. Change in temperaturet and moisture
More informationMechanics of Composite Materials, Second Edition Autar K Kaw University of South Florida, Tampa, USA
Mechanics of Composite Materials, Second Edition Autar K Kaw University of South Florida, Tampa, USA What programs are in PROMAL? Master Menu The master menu screen with five separate applications from
More informationModule 5: Laminate Theory Lecture 17: Laminate Constitutive Relations. The Lecture Contains: Laminate Constitutive Relations
Lecture 17: Laminate Constitutive Relations The Lecture Contains: Laminate Constitutive Relations Classification of Laminates CrossPly Laminates Specially Orthotropic Laminates Examples Homework References
More informationTABLE OF CONTENTS. Mechanics of Composite Materials, Second Edition Autar K Kaw University of South Florida, Tampa, USA
Mechanics of Composite Materials, Second Edition Autar K Kaw University of South Florida, Tampa, USA TABLE OF CONTENTS 1. INTRODUCTION TO COMPOSITE MATERIALS 1.1 Introduction... 1.2 Classification... 1.2.1
More informationBending of Simply Supported Isotropic and Composite Laminate Plates
Bending of Simply Supported Isotropic and Composite Laminate Plates Ernesto GutierrezMiravete 1 Isotropic Plates Consider simply a supported rectangular plate of isotropic material (length a, width b,
More informationChapter 2  Macromechanical Analysis of a Lamina. Exercise Set. 2.1 The number of independent elastic constants in three dimensions are: 2.
Chapter  Macromechanical Analysis of a Lamina Exercise Set. The number of independent elastic constants in three dimensions are: Anisotropic Monoclinic 3 Orthotropic 9 Transversely Orthotropic 5 Isotropic.
More informationFig. 1. Circular fiber and interphase between the fiber and the matrix.
Finite element unit cell model based on ABAQUS for fiber reinforced composites Tian Tang Composites Manufacturing & Simulation Center, Purdue University West Lafayette, IN 47906 1. Problem Statement In
More informationComputational Analysis for Composites
Computational Analysis for Composites Professor Johann Sienz and Dr. Tony Murmu Swansea University July, 011 The topics covered include: OUTLINE Overview of composites and their applications Micromechanics
More informationLecture 8. Stress Strain in Multidimension
Lecture 8. Stress Strain in Multidimension Module. General Field Equations General Field Equations [] Equilibrium Equations in Elastic bodies xx x y z yx zx f x 0, etc [2] Kinematics xx u x x,etc. [3]
More informationPassive Damping Characteristics of Carbon Epoxy Composite Plates
Journal of Materials Science and Engineering A 6 () 354 doi:.765/663/6..5 D DAVID PUBLISHING Passive Damping Characteristics of Carbon Epoxy Composite Plates Dileep Kumar K * and V V Subba Rao Faculty
More informationStress, Strain Stress strain relationships for different types of materials Stress strain relationships for a unidirectional/bidirectional lamina
Chapter 2 Macromechanical Analysis of a Lamina Stress, Strain Stress strain relationships for different types of materials Stress strain relationships for a unidirectional/bidirectional lamina Islamic
More informationModule 7: Micromechanics Lecture 25: Strength of Materials Approach. Introduction. The Lecture Contains. Effective Transverse Modulus
Introduction In the previous lecture we have introduced the concept of Representative Volume Element or Unit Cell. This is the basic building block in a micromechanical study. Further, we explained the
More informationUnderstand basic stressstrain response of engineering materials.
Module 3 Constitutive quations Learning Objectives Understand basic stressstrain response of engineering materials. Quantify the linear elastic stressstrain response in terms of tensorial quantities
More informationInfluence of the filament winding process variables on the mechanical behavior of a composite pressure vessel
Influence of the filament winding process variables on the mechanical behavior of a composite pressure vessel G. Vargas 1 & A. Miravete 2 1 Universidad Pontificia Bolivariana, Facultad de Ingeniería Mecánica,
More informationCrash and Impact Simulation of Composite Structures by Using CAE Process Chain
Crash and Impact Simulation of Composite Structures by Using CAE Process Chain Madhukar Chatiri 1, Thorsten Schütz 2, Anton Matzenmiller 3, Ulrich Stelzmann 1 1 CADFEM GmbH, Grafing/Munich, Germany, mchatiri@cadfem.de
More informationEffect of Thermal Stresses on the Failure Criteria of Fiber Composites
Effect of Thermal Stresses on the Failure Criteria of Fiber Composites Martin Leong * Institute of Mechanical Engineering Aalborg University, Aalborg, Denmark Bhavani V. Sankar Department of Mechanical
More informationThe stiffness of plates
The stiffness of plates 1. Introduction The word plate is a collective term for elements in which forces can be transferred in two directions. Floors, walls, bridge slabs and laminates are all plates.
More informationMaterials and Structures. Indian Institute of Technology Kanpur
Introduction to Composite Materials and Structures Nachiketa Tiwari Indian Institute of Technology Kanpur Lecture 34 Thermal Stresses in Plates Lecture Overview Introduction Mechanical and Thermal Strains
More informationComposite models 30 and 131: Ply types 0 and 8 calibration
Model calibration Composite BiPhase models 30 and 3 for elastic, damage and failure PAMCRASH material model 30 is for solid and 3 for multilayered shell elements. Within these models different ply types
More informationModule 7: Micromechanics Lecture 34: Self Consistent, Mori Tanaka and Halpin Tsai Models. Introduction. The Lecture Contains. Self Consistent Method
Introduction In this lecture we will introduce some more micromechanical methods to predict the effective properties of the composite. Here we will introduce expressions for the effective properties without
More informationAnalysis of Composite Pressure Vessels
Analysis of Composite Pressure Vessels Reza Mohammadzadeh Gheshlaghi 1 Mohammad Hassan Hojjati Hamid Reza Mohammadi Daniali 3 1 Engineering Research Centre, Tabriz, Iran,3 Department of Mechanical Engineering,
More informationModule 3: 3D Constitutive Equations Lecture 10: Constitutive Relations: Generally Anisotropy to Orthotropy. The Lecture Contains: Stress Symmetry
The Lecture Contains: Stress Symmetry Strain Symmetry Strain Energy Density Function Material Symmetry Symmetry with respect to a Plane Symmetry with respect to two Orthogonal Planes Homework References
More informationLectures on. Constitutive Modelling of Arteries. Ray Ogden
Lectures on Constitutive Modelling of Arteries Ray Ogden University of Aberdeen Xi an Jiaotong University April 2011 Overview of the Ingredients of Continuum Mechanics needed in Soft Tissue Biomechanics
More informationSmart Materials, Adaptive Structures, and Intelligent Mechanical Systems
Smart Materials, Adaptive Structures, and Intelligent Mechanical Systems Bishakh Bhattacharya & Nachiketa Tiwari Indian Institute of Technology Kanpur Lecture 19 Analysis of an Orthotropic Ply References
More informationCoupling of plasticity and damage in glass fibre reinforced polymer composites
EPJ Web of Conferences 6, 48 1) DOI: 1.151/epjconf/1648 c Owned by the authors, published by EDP Sciences, 1 Coupling of plasticity and damage in glass fibre reinforced polymer composites R. Kvale Joki
More informationVIBRATION AND DAMPING ANALYSIS OF FIBER REINFORCED COMPOSITE MATERIAL CONICAL SHELLS
VIBRATION AND DAMPING ANALYSIS OF FIBER REINFORCED COMPOSITE MATERIAL CONICAL SHELLS Mechanical Engineering Department, Indian Institute of Technology, New Delhi 110 016, India (Received 22 January 1992,
More informationModelling of multiaxial ultimate elastic wall stress (UEWS) test for glass fibre reinforced epoxy (GRE) composite pipes
pplied Mechanics and Materials Vol. 367 (013) pp 113117 Online available since 013/ug/16 at www.scientific.net (013) Trans Tech Publications, Switzerland doi:10.408/www.scientific.net/mm.367.113 Modelling
More informationELASTICITY (MDM 10203)
LASTICITY (MDM 10203) Lecture Module 5: 3D Constitutive Relations Dr. Waluyo Adi Siswanto University Tun Hussein Onn Malaysia Generalised Hooke's Law In one dimensional system: = (basic Hooke's law) Considering
More information2.1 Strain energy functions for incompressible materials
Chapter 2 Strain energy functions The aims of constitutive theories are to develop mathematical models for representing the real behavior of matter, to determine the material response and in general, to
More informationA HIGHERORDER BEAM THEORY FOR COMPOSITE BOX BEAMS
A HIGHERORDER BEAM THEORY FOR COMPOSITE BOX BEAMS A. Kroker, W. Becker TU Darmstadt, Department of Mechanical Engineering, Chair of Structural Mechanics Hochschulstr. 1, D64289 Darmstadt, Germany kroker@mechanik.tudarmstadt.de,
More informationDEVELOPMENT OF A MICROMECHANICAL MODEL IN INTERACTION WITH PARAMETERS RELATED TO THE MICROSTRUCTURE OF CARBON/EPOXY COMPOSITES
ECCM1616 TH EUROPEAN CONFERENCE ON COMPOSITE MATERIALS, Seville, Spain, 2226 June 2014 DEVELOPMENT OF A MICROMECHANICAL MODEL IN INTERACTION WITH PARAMETERS RELATED TO THE MICROSTRUCTURE OF CARBON/EPOXY
More informationAdvanced Structural Analysis EGF Section Properties and Bending
Advanced Structural Analysis EGF316 3. Section Properties and Bending 3.1 Loads in beams When we analyse beams, we need to consider various types of loads acting on them, for example, axial forces, shear
More informationME 7502 Lecture 2 Effective Properties of Particulate and Unidirectional Composites
ME 75 Lecture Effective Properties of Particulate and Unidirectional Composites Concepts from Elasticit Theor Statistical Homogeneit, Representative Volume Element, Composite Material Effective Stress
More informationLAMINATED COMPOSITE PLATES
LAMINATED COMPOSITE PLATES David Roylance Department of Materials Science and Engineering Massachusetts Institute of Technology Cambridge, MA 02139 February 10, 2000 Introduction This document is intended
More informationASSESSMENT OF MIXED UNIFORM BOUNDARY CONDITIONS FOR PREDICTING THE MACROSCOPIC MECHANICAL BEHAVIOR OF COMPOSITE MATERIALS
ASSESSMENT OF MIXED UNIFORM BOUNDARY CONDITIONS FOR PREDICTING THE MACROSCOPIC MECHANICAL BEHAVIOR OF COMPOSITE MATERIALS Dieter H. Pahr and Helmut J. Böhm Institute of Lightweight Design and Structural
More informationStacking sequences for Extensionally Isotropic, Fully Isotropic and QuasiHomogeneous Orthotropic Laminates.
49th AIAA/ASME/ASCE/AHS/ASC Structures, Structural Dynamics, and Materials 710 April 2008, Schaumburg, IL AIAA 20081940 Stacking sequences for Extensionally Isotropic, Fully Isotropic and QuasiHomogeneous
More information16.20 HANDOUT #2 Fall, 2002 Review of General Elasticity
6.20 HANDOUT #2 Fall, 2002 Review of General Elasticity NOTATION REVIEW (e.g., for strain) Engineering Contracted Engineering Tensor Tensor ε x = ε = ε xx = ε ε y = ε 2 = ε yy = ε 22 ε z = ε 3 = ε zz =
More informationMaterials and Structures. Indian Institute of Technology Kanpur
Introduction to Composite Materials and Structures Nachiketa Tiwari Indian Institute of Technology Kanpur Lecture 15 Behavior of Unidirectional Composites Lecture Overview Mt Material ilaxes in unidirectional
More informationModule 4: Behaviour of a LaminaeII. Learning Unit 1: M1. M4.1 Mechanics of Composites. M4.1.1 Introduction to Mechanics of Composites
Module 4: Behaviour of a LaminaeII Learning Unit 1: M1 M4.1 Mechanics of Composites M4.1.1 Introduction to Mechanics of Composites The relation between ply uniaxial strengths and constituent properties
More informationINTERNATIONAL JOURNAL OF APPLIED ENGINEERING RESEARCH, DINDIGUL Volume 2, No 1, 2011
Interlaminar failure analysis of FRP cross ply laminate with elliptical cutout Venkateswara Rao.S 1, Sd. Abdul Kalam 1, Srilakshmi.S 1, Bala Krishna Murthy.V 2 1 Mechanical Engineering Department, P. V.
More informationA synergistic damage mechanics approach to mechanical response of composite laminates with ply cracks
Article A synergistic damage mechanics approach to mechanical response of composite laminates with ply cracks JOURNAL OF COMPOSITE MATERIALS Journal of Composite Materials 0(0) 7! The Author(s) 0 Reprints
More informationGetting Started with Composites Modeling and Analysis
Getting Started with Composites Modeling and Analysis IN THIS WEBINAR: PRESENTED BY: Orthotropic materials and how to define them Composite Laminate properties and modeling Composite failure theories and
More informationModule 7: Micromechanics Lecture 29: Background of Concentric Cylinder Assemblage Model. Introduction. The Lecture Contains
Introduction In this lecture we are going to introduce a new micromechanics model to determine the fibrous composite effective properties in terms of properties of its individual phases. In this model
More informationEFFECT OF LAMINATION ANGLE AND THICKNESS ON ANALYSIS OF COMPOSITE PLATE UNDER THERMO MECHANICAL LOADING
Journal of MECHANICAL ENGINEERING Strojnícky časopis, VOL 67 (217), NO 1, 522 EFFECT OF LAMINATION ANGLE AND THICKNESS ON ANALYSIS OF COMPOSITE PLATE UNDER THERMO MECHANICAL LOADING Arnab Choudhury 1,
More informationMechanical Behavior of Circular Composite Springs with Extended Flat Contact Surfaces
Mechanical Behavior of Circular Composite Springs with Extended Flat Contact Surfaces PingCheung Tse epartment of Mechanical Engineering, The Hong Kong Polytechnic University, Hunghom, Kowloon, Hong Kong
More informationFINITE ELEMENT AND EXPERIMENTAL STUDY OF NOVEL CONCEPT OF 3D FIBRE CELL STRUCTURE
FINITE ELEMENT AND EXPERIMENTAL STUDY OF NOVEL CONCEPT OF 3D FIBRE CELL STRUCTURE M. Růžička, V. Kulíšek 2, J. Had, O. Prejzek Department of Mechanics, Biomechanics and Mechatronics, Faculty of Mechanical
More informationPassive Damping Characteristics of Carbon Epoxy Composite Plates
Journal of aterials Science and Engineering A 6 (12) (2016) 3542 doi: 10.17265/21616213/2016.12.005 D DAVID PUBLISHIG Passive Damping Characteristics of Carbon Epoxy Composite Plates Dileep Kumar K
More informationCrashworthy Design of Composite Structures Using CAE Process Chain
0 th European LSDYNA Conference 205, Würzburg, Germany Crashworthy Design of Composite Structures Using CAE Process Chain Madhukar Chatiri, Thorsten Schuetz 2, Anton Matzenmiller 3 CADFEM GmbH, Grafing
More informationFundamentals of Linear Elasticity
Fundamentals of Linear Elasticity Introductory Course on Multiphysics Modelling TOMASZ G. ZIELIŃSKI bluebox.ippt.pan.pl/ tzielins/ Institute of Fundamental Technological Research of the Polish Academy
More informationMATERIAL MECHANICS, SE2126 COMPUTER LAB 4 MICRO MECHANICS. E E v E E E E E v E E + + = m f f. f f
MATRIAL MCHANICS, S226 COMPUTR LAB 4 MICRO MCHANICS 2 2 2 f m f f m T m f m f f m v v + + = + PART A SPHRICAL PARTICL INCLUSION Consider a solid granular material, a so called particle composite, shown
More informationA copy can be downloaded for personal noncommercial research or study, without prior permission or charge
York, C. B. (2015) Influence of bending twisting coupling on compression and shear buckling strength. Stability of Structures 14th Symposium, Zakopane, Poland, 812 Jun 2015. Copyright 2015 The Author.
More informationElements of Continuum Elasticity. David M. Parks Mechanics and Materials II February 25, 2004
Elements of Continuum Elasticity David M. Parks Mechanics and Materials II 2.002 February 25, 2004 Solid Mechanics in 3 Dimensions: stress/equilibrium, strain/displacement, and intro to linear elastic
More informationUSING A HOMOGENIZATION PROCEDURE FOR PREDICTION OF MATERIAL PROPERTIES AND THE IMPACT RESPONSE OF UNIDIRECTIONAL COMPOSITE
Volume II: Fatigue, Fracture and Ceramic Matrix Composites USING A HOMOGENIZATION PROCEDURE FOR PREDICTION OF MATERIAL PROPERTIES AND THE IMPACT RESPONSE OF UNIDIRECTIONAL COMPOSITE A. D. Resnyansky and
More information16.21 Techniques of Structural Analysis and Design Spring 2003 Unit #5  Constitutive Equations
6.2 Techniques of Structural Analysis and Design Spring 2003 Unit #5  Constitutive quations Constitutive quations For elastic materials: If the relation is linear: Û σ ij = σ ij (ɛ) = ρ () ɛ ij σ ij =
More informationON THE NUMERICAL ANALYSIS OF COMPOSITE MATERIAL
The 4th International Conference Advanced Composite Materials Engineering COMAT 8 October, Brasov, Romania O THE UMERICAL AALYSIS OF COMPOSITE MATERIAL D.D. icoara Transilvania University, City Brasov,
More informationMost of the material in this package is based on a recently published book. This is:
Mechanics of Composite Materials Version 2.1 Bill Clyne, University of Cambridge Boban Tanovic, MATTER Assumed Preknowledge It is assumed that the student is familiar with simple concepts of mechanical
More informationElasticity in two dimensions 1
Elasticity in two dimensions 1 Elasticity in two dimensions Chapters 3 and 4 of Mechanics of the Cell, as well as its Appendix D, contain selected results for the elastic behavior of materials in two and
More informationTrace a gamechanging discovery
Trace a gamechanging discovery Stephen W. Tsai Stanford University October 5, 2015 Topics Why trace? The one and only unifying constant Theory of trace simple; easy to understand CPly by Stanford/Chomarat
More informationA Constitutive Framework for the Numerical Analysis of Organic Soils and Directionally Dependent Materials
Dublin, October 2010 A Constitutive Framework for the Numerical Analysis of Organic Soils and Directionally Dependent Materials FracMan Technology Group Dr Mark Cottrell Presentation Outline Some Physical
More informationFRACTURE TOUGHNESS OF ADHESIVE BONDED COMPOSITE JOINTS UNDER MIXED MODE LOADING.
FRACTURE TOUGHNESS OF ADHESIVE BONDED COMPOSITE JOINTS UNDER MIXED MODE LOADING. X. J. Gong, F. Hernandez, G. Verchery. ISAT  Institut Supérieur de l Automobile et des Transports, LRMA  Laboratoire de
More informationMechanical and Thermal Properties of Coir Fiber Reinforced Epoxy Composites Using a Micromechanical Approach
Mechanical and Thermal Properties of Coir Fiber Reinforced Epoxy Composites Using a Micromechanical Approach Sandhyarani Biswas Department of Mechanical Engineering, N.I.T Rourkela, INDIA Abstract: Nowadays,
More informationOpenhole compressive strength prediction of CFRP composite laminates
Openhole compressive strength prediction of CFRP composite laminates O. İnal 1, A. Ataş 2,* 1 Department of Mechanical Engineering, Balikesir University, Balikesir, 10145, Turkey, inal@balikesir.edu.tr
More informationCHEME2200: Polymer blends and composites Fibre architecture and principles of reinforcement
CHEME2200: Polymer blends and composites Fibre architecture and principles of reinforcement Mark Hughes 19 th September 2016 Outline Fibre architecture Volume fraction and the rule of mixtures Principle
More informationME 582 Advanced Materials Science. Chapter 2 Macromechanical Analysis of a Lamina (Part 2)
ME 582 Advanced Materials Science Chapter 2 Macromechanical Analysis of a Lamina (Part 2) Laboratory for Composite Materials Research Department of Mechanical Engineering University of South Alabama, Mobile,
More informationExercise: concepts from chapter 8
Reading: Fundamentals of Structural Geology, Ch 8 1) The following exercises explore elementary concepts associated with a linear elastic material that is isotropic and homogeneous with respect to elastic
More informationN = Shear stress / Shear strain
UNIT  I 1. What is meant by factor of safety? [A/M15] It is the ratio between ultimate stress to the working stress. Factor of safety = Ultimate stress Permissible stress 2. Define Resilience. [A/M15]
More informationFinite element modelling of infinitely wide Angleply FRP. laminates
www.ijaser.com 2012 by the authors Licensee IJASER Under Creative Commons License 3.0 editorial@ijaser.com Research article ISSN 2277 9442 Finite element modelling of infinitely wide Angleply FRP laminates
More information8 Properties of Lamina
8 Properties of Lamina 8 ORTHOTROPIC LAMINA An orthotropic lamina is a sheet with unique and predictable properties and consists of an assemblage of fibers ling in the plane of the sheet and held in place
More informationEffect of Specimen Dimensions on Flexural Modulus in a 3Point Bending Test
Effect of Specimen Dimensions on Flexural Modulus in a 3Point Bending Test M. Praveen Kumar 1 and V. Balakrishna Murthy 2* 1 Mechanical Engineering Department, P.V.P. Siddhartha Institute of Technology,
More informationSIMULATION OF PROGRESSIVE FAILURE PREDICTION OF FILAMENT WOUND COMPOSITE TUBES SUBJECTED TO MULTIPLE LOADING WITH MEMBRANEFLEXION COUPLING EFFECTS
VOL. 5, NO. 4, APRIL 010 ISSN 18196608 006010 Asian Research Publishing Network (ARPN). All rights reserved. SIMULATION OF PROGRESSIVE FAILURE PREDICTION OF FILAMENT WOUND COMPOSITE TUBES SUBJECTED TO
More informationNonconventional Glass fiber NCF composites with thermoset and thermoplastic matrices. F Talence, France Le Cheylard, France
20 th International Conference on Composite Materials Copenhagen, 1924th July 2015 Nonconventional Glass fiber NCF composites with thermoset and thermoplastic matrices. Thierry Lorriot 1, Jalal El Yagoubi
More informationFracture Mechanics, Damage and Fatigue: Composites
University of Liège Aerospace & Mechanical Engineering Fracture Mechanics, Damage and Fatigue: Composites Ludovic Noels Computational & Multiscale Mechanics of Materials CM3 http://www.ltascm3.ulg.ac.be/
More informationComposites Design and Analysis. Stress Strain Relationship
Composites Design and Analysis Stress Strain Relationship Composite design and analysis Laminate Theory Manufacturing Methods Materials Composite Materials Design / Analysis Engineer Design Guidelines
More informationMECH 5312 Solid Mechanics II. Dr. Calvin M. Stewart Department of Mechanical Engineering The University of Texas at El Paso
MECH 5312 Solid Mechanics II Dr. Calvin M. Stewart Department of Mechanical Engineering The University of Texas at El Paso Table of Contents Thermodynamics Derivation Hooke s Law: Anisotropic Elasticity
More information3D Elasticity Theory
3D lasticity Theory Many structural analysis problems are analysed using the theory of elasticity in which Hooke s law is used to enforce proportionality between stress and strain at any deformation level.
More informationISSN: ISO 9001:2008 Certified International Journal of Engineering Science and Innovative Technology (IJESIT) Volume 2, Issue 4, July 2013
Delamination Studies in FibreReinforced Polymer Composites K.Kantha Rao, Dr P. Shailesh, K. Vijay Kumar 1 Associate Professor, Narasimha Reddy Engineering College Hyderabad. 2 Professor, St. Peter s Engineering
More informationMATERIAL ELASTIC ANISOTROPIC command
MATERIAL ELASTIC ANISOTROPIC command.. Synopsis The MATERIAL ELASTIC ANISOTROPIC command is used to specify the parameters associated with an anisotropic linear elastic material idealization. Syntax The
More informationMECHANICAL CHARACTERISTICS OF CARBON FIBER YACHT MASTS
MECHANICAL CHARACTERISTICS OF CARBON FIBER YACHT MASTS This paper provides a preliminary stress analysis of a carbon reinforced layered cylinder such as would be found in a yacht mast. The cylinder is
More informationCalculation of Damagedependent Directional Failure Indices from the TsaiWu Static Failure Criterion
Van Paepegem, W. and Degrieck, J. (3. alculation of Damagedependent Directional Failure Indices from the saiwu Static Failure riterion. omposites Science and echnology, 63(, 353. alculation of Damagedependent
More informationBasic concepts to start Mechanics of Materials
Basic concepts to start Mechanics of Materials Georges Cailletaud Centre des Matériaux Ecole des Mines de Paris/CNRS Notations Notations (maths) (1/2) A vector v (element of a vectorial space) can be seen
More informationSTRUCTURAL EFFICIENCY VIA MINIMISATION OF ELASTIC ENERGY IN DAMAGE TOLERANT LAMINATES
ECCM1616 TH EUROPEAN CONFERENCE ON COMPOSITE MATERIALS, Seville, Spain, 2226 June 214 STRUCTURAL EFFICIENCY VIA MINIMISATION OF ELASTIC ENERGY IN DAMAGE TOLERANT LAMINATES M. Nielsen a, A. T. Rhead a,
More informationThe Power of Ultrasonic Characterisation for Completely Assessing the Elastic Properties of Materials
11th European Conference on NonDestructive Testing (ECNDT 214), October 61, 214, Prague, Czech Republic The Power of Ultrasonic Characterisation for Completely Assessing the Elastic Properties of Materials
More informationLAMINATED COMPOSITE PLATES
LAMINATED COMPOSITE PLATES David Roylance Department of Materials Science and Engineering Massachusetts Institute of Technology Cambridge, MA 02139 February 10, 2000 Introduction This document is intended
More informationMATERIAL PROPERTIES. Material Properties Must Be Evaluated By Laboratory or Field Tests 1.1 INTRODUCTION 1.2 ANISOTROPIC MATERIALS
. MARIAL PROPRIS Material Properties Must Be valuated By Laboratory or Field ests. INRODUCION he fundamental equations of structural mechanics can be placed in three categories[]. First, the stressstrain
More informationA FINITE ELEMENT MODEL TO PREDICT MULTI AXIAL STRESSSTRAIN RESPONSE OF CERAMIC MATRIX COMPOSITES WITH STRAIN INDUCED DAMAGE
A FINITE ELEMENT MODEL TO PREDICT MULTI AXIAL STRESSSTRAIN RESPONSE OF CERAMIC MATRIX COMPOSITES WITH STRAIN INDUCED DAMAGE Daxu Zhang and D. R. Hayhurst School of Mechanical, Aerospace and Civil Engineering,
More informationBuckling Behavior of 3D Randomly Oriented CNT Reinforced Nanocomposite Plate
Buckling Behavior of 3D Randomly Oriented CNT Reinforced Nanocomposite Plate Outline Introduction Representative Volume Element (RVE) Periodic Boundary Conditions on RVE Homogenization Method Analytical
More informationTHE TRANSVERSE OFFAXIS STIFFNESS AND STRENGTH OF SOFTWOODS. Abstract
THE TRANSVERSE OFFAXIS STIFFNESS AND STRENGTH OF SOFTWOODS Carl S. Moden 1, Jessica Polycarpe 1 and Lars A. Berglund 2 1 Dept. of Aeronautical and Vehicle Engineering The Royal Institute of Technology
More informationOnline publication date: 23 October 2010
This article was downloaded by: [informa internal users] On: 1 November 2010 Access details: Access Details: [subscription number 755239602] Publisher Taylor & Francis Informa Ltd Registered in England
More information